ASTM-D5571 › Historical Revision Information
Standard Test Method for Environmental Stress Crack Resistance (ESCR) of Plastic Tighthead Drums Not Exceeding 60 Gal (227 L) in Rated Capacity
Show Complete Document History
The following bibliographic material is provided to assist you with your purchasing decision:
1.1 This test method provides an indication of the environmental stress crack resistance of plastic tighthead drums as a summation of the effects of container design, resin, manufacturing conditions, field performance, and other factors.
1.2 This test method may be used to evaluate a plastic drum's resistance to failure by cracking when in the presence of chemical and physical stresses.
1.3 Two procedures are provided as follows:
1.3.1 Procedure A—Internal pressure stress crack resistance method to nonyl phenoxypoly (ethyleneoxy) ethanol solution, a stress cracking reagent. The internal pressure is controlled at a constant elevated pressure and temperature.
1.3.2 Procedure B—Top-load stress crack resistance method to nonyl phenoxypoly ethanol, a stress cracking reagent. The compressive top load is controlled at a constant weight while maintaining an elevated temperature.
1.4 Although these procedures are not designed to test the ability of the closure or closure gasket material to retain the test reagent, the inclusion of closure failure as a container failure mode is optional. However, leakage through a closure may affect the internal pressure that could affect the test results.
1.5 This test method does not attempt to address all factors that could lead to stress cracking of plastic drums. The user of this standard may use other test parameters, such as top loads, chemical reagents, etc., as agreed upon between the user and supplier in the event of a drum qualification or purchase agreement.
1.6 The values stated in inch-pound units are to be regarded as the standard. The SI units given in parentheses are for information only.
1.7 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. Specific warning statements are given in 6.2.
Significance and Use
These procedures provide an indication of the environmental stress-crack resistance of plastic tighthead drums. This test method may be used for determining the applicability of various plastic resins, mold designs, processing techniques and parameters for plastic tighthead drums.
Environmental stress cracking is indicative of what results when a container is exposed to chemical agents such as soaps, organics, bleaches, or any surface active solutions while under conditions of stress.
Environmental stress cracking is a mechanism of chemical attack that is highly dependent upon the test reagent, resin, drum manufacturing or processing history, exposure temperature, and applied stress. The combination of these factors may result in eventual stress crack failure.
Both procedures minimize the potential for test variability by providing the user with rigidly defined test conditions. This test method may be used as design qualification and auditing tools for plastic tighthead drums.
This test method is not meant to provide a quantitative value of measurement (that is, number of days to failure). It is intended only as a pass/fail procedure in accordance with user's specifications, or as agreed upon between the user and supplier. It is not intended as a predictor or indicator of field performance regarding time to failure.
drum; environmental stress crack; internal pressure; plastic; stacking; stress crack; tighthead; Stress--plastics; Stress cracking tests; Tighthead drum; Drums; Environmental stress crack resistance (ESCR); Internal pressure/testing; Plastic shipping materials/applications; Pressure testing--packaging/containers; Shipping containers/materials/applications; Stacking test; Stress--environmental effects; ICS Number Code 55.140 (Barrels. Drums. Canisters)
To find similar documents by ASTM Volume:
15.10 (Packaging; Flexible Barrier Packaging)
To find similar documents by classification:
55.140 (Barrels. Drums. Canisters Containers mainly for transportation of fluids, including also casks, pails, large tin cans for shipping materials, etc. Fluid storage devices, see 23.020)
This document comes with our free Notification Service, good for the life of the document.
This document is available in either Paper or PDF format.
1994 R10 EDITION
May 1, 2010